Wet-Environment-Induced Structural Alterations in Single- and Polycrystalline LLZTO Solid Electrolytes Studied by Diffraction Techniques
Redhammer, Günther J.; Badami, Pavan; Meven, Martin; Ganschow, Steffen; Berendts, Stefan; Tippelt, Gerold; Rettenwander, Daniel; ACS Applied Materials & Interfaces  (2020) –; doi:10.1021/acsami.0c16016

data_4518348
_publ_section_title
;
 Wet-Environment-Induced Structural Alterations in Single- and
 Polycrystalline LLZTO Solid Electrolytes Studied by Diffraction
 Techniques
;
_journal_name_full               'ACS Applied Materials &amp; Interfaces'
_journal_paper_doi               10.1021/acsami.0c16016
_journal_year                    2020
_chemical_absolute_configuration unk
_chemical_formula_moiety         'La2.95 Li3.73 H1.57 Ta1.10 Zr0.90 O12'
_chemical_formula_sum            'H1.57 La2.95 Li3.73 O12 Ta1.1 Zr0.9'
_chemical_formula_weight         913.03
_space_group_IT_number           220
_space_group_name_Hall           'I -4bd 2c 3'
_space_group_name_H-M_alt        'I -4 3 d'
_symmetry_cell_setting           cubic
_symmetry_Int_Tables_number      220
_symmetry_space_group_name_Hall  'I -4bd 2c 3'
_symmetry_space_group_name_H-M   'I -4 3 d'
_atom_sites_solution_hydrogens   difmap
_audit_conform_dict_location     ftp://ftp.iucr.org/pub/cif_core.dic
_audit_conform_dict_name         cif_core.dic
_audit_conform_dict_version      2.4.5
_audit_creation_date             2020-05-29T12:06:45-00:00
_audit_creation_method           'WinGX routine CIF_UPDATE'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            8
_cell_length_a                   12.9466(3)
_cell_length_b                   12.9466(3)
_cell_length_c                   12.9466(3)
_cell_measurement_reflns_used    33706
_cell_measurement_temperature    293(2)
_cell_measurement_theta_max      36.427
_cell_measurement_theta_min      3.855
_cell_measurement_wavelength     0.71073
_cell_volume                     2170.04(9)
_computing_cell_refinement       'Bruker APEX2 (Bruker, 2012)'
_computing_data_collection       'Bruker APEX2 (Bruker, 2012)'
_computing_data_reduction        'Bruker APEX2 (Bruker, 2012)'
_computing_molecular_graphics    'Diamonds 3.2g (Brandenburg,2006)'
_computing_publication_material  'WinGX v1.70.01 (Farrugia 2012)'
_computing_structure_refinement  'SHELXL-2012 (Sheldrick, 2012)'
_computing_structure_solution    'SHELXS-2012 (Sheldrick, 2012)'
_diffrn_ambient_temperature      293(2)
_diffrn_measured_fraction_theta_full 1
_diffrn_measured_fraction_theta_max 0.998
_diffrn_measurement_device       '3-circle diffractometer'
_diffrn_measurement_device_type  'SMART APEX'
_diffrn_measurement_method
'rotation, \w-scans at 4 different \f positions'
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_probe          x-ray
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0534
_diffrn_reflns_av_unetI/netI     0.0134
_diffrn_reflns_Laue_measured_fraction_full 1
_diffrn_reflns_Laue_measured_fraction_max 0.998
_diffrn_reflns_limit_h_max       21
_diffrn_reflns_limit_h_min       -21
_diffrn_reflns_limit_k_max       21
_diffrn_reflns_limit_k_min       -21
_diffrn_reflns_limit_l_max       21
_diffrn_reflns_limit_l_min       -21
_diffrn_reflns_number            33706
_diffrn_reflns_point_group_measured_fraction_full 1
_diffrn_reflns_point_group_measured_fraction_max 0.999
_diffrn_reflns_theta_full        25.242
_diffrn_reflns_theta_max         36.427
_diffrn_reflns_theta_min         3.855
_exptl_absorpt_coefficient_mu    23.348
_exptl_absorpt_correction_T_max  0.210
_exptl_absorpt_correction_T_min  0.065
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details
'multiscan correction with APEX2 software (Bruker 2012)'
_exptl_crystal_colour            colourless
_exptl_crystal_density_diffrn    5.589
_exptl_crystal_density_method    'not measured'
_exptl_crystal_description       plate
_exptl_crystal_F_000             3161.0
_exptl_crystal_size_max          0.14
_exptl_crystal_size_mid          0.13
_exptl_crystal_size_min          0.07
_refine_diff_density_max         0.917
_refine_diff_density_min         -0.739
_refine_diff_density_rms         0.145
_refine_ls_abs_structure_details
;
 Refined as an inversion twin.
;
_refine_ls_abs_structure_Flack   0.58(6)
_refine_ls_extinction_coef       0.000307(18)
_refine_ls_extinction_expression Fc^*^=kFc[1+0.001xFc^2^\l^3^/sin(2\q)]^-1/4^
_refine_ls_extinction_method     'SHELXL-2014/7 (Sheldrick 2014'
_refine_ls_goodness_of_fit_ref   1.185
_refine_ls_hydrogen_treatment    refxyz
_refine_ls_matrix_type           full
_refine_ls_number_constraints    0
_refine_ls_number_parameters     50
_refine_ls_number_reflns         888
_refine_ls_number_restraints     8
_refine_ls_restrained_S_all      1.189
_refine_ls_R_factor_all          0.0163
_refine_ls_R_factor_gt           0.0161
_refine_ls_shift/su_max          0.008
_refine_ls_shift/su_mean         0.001
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'w=1/[\s^2^(Fo^2^)+17.6898P] where P=(Fo^2^+2Fc^2^)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0325
_refine_ls_wR_factor_ref         0.0326
_reflns_Friedel_coverage         0.813
_reflns_Friedel_fraction_full    1
_reflns_Friedel_fraction_max     1
_reflns_number_gt                885
_reflns_number_total             888
_reflns_threshold_expression     'I > 2\s(I)'
_cod_data_source_file            am0c16016_si_004.cif
_cod_data_source_block           CZ_LLZTO_363k_1d
_cod_original_cell_volume        2170.04(15)
_cod_original_formula_sum        'La2.95 Li3.73 H1.57 Ta1.10 Zr0.90 O12'
_cod_database_code               4518348
_shelx_shelxl_version_number     2014/7